The material described by Li4Co3Cu3(TeO8)2 is Hausmannite-derived structured and crystallizes in the triclinic P1 space group. There are four inequivalent Li sites. In the first Li site, Li(1) is bonded to one O(11), one O(12), one O(15), and one O(3) atom to form LiO4 tetrahedra that share  a cornercorner with one Co(1)O6 octahedra,  a cornercorner with one Cu(1)O6 octahedra,  a cornercorner with one Cu(2)O6 octahedra, corners with two equivalent Co(2)O6 octahedra, corners with two equivalent Co(3)O6 octahedra, corners with two equivalent Cu(3)O6 octahedra, and corners with three equivalent Te(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 53-68°. In the second Li site, Li(2) is bonded to one O(14), one O(16), one O(5), and one O(9) atom to form distorted LiO4 tetrahedra that share  a cornercorner with one Co(2)O6 octahedra,  a cornercorner with one Co(3)O6 octahedra,  a cornercorner with one Cu(3)O6 octahedra, corners with three equivalent Te(2)O6 octahedra,  an edgeedge with one Co(1)O6 octahedra,  an edgeedge with one Cu(1)O6 octahedra, and  an edgeedge with one Cu(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 56-68°. In the third Li site, Li(3) is bonded in a rectangular see-saw-like geometry to one O(1), one O(10), one O(4), and one O(6) atom. In the fourth Li site, Li(4) is bonded to one O(13), one O(2), one O(7), and one O(8) atom to form LiO4 tetrahedra that share  a cornercorner with one Co(2)O6 octahedra,  a cornercorner with one Co(3)O6 octahedra,  a cornercorner with one Cu(3)O6 octahedra, corners with two equivalent Co(1)O6 octahedra, corners with two equivalent Cu(1)O6 octahedra, corners with two equivalent Cu(2)O6 octahedra, and corners with three equivalent Te(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 50-68°. There are three inequivalent Co sites. In the first Co site, Co(1) is bonded to one O(14), one O(16), one O(3), one O(4), one O(7), and one O(8) atom to form CoO6 octahedra that share corners with two equivalent Te(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  an edgeedge with one Te(1)O6 octahedra, edges with two equivalent Cu(1)O6 octahedra, edges with two equivalent Cu(2)O6 octahedra, and  an edgeedge with one Li(2)O4 tetrahedra. The corner-sharing octahedral tilt angles range from 45-48°. In the second Co site, Co(2) is bonded to one O(1), one O(10), one O(11), one O(13), one O(15), and one O(5) atom to form CoO6 octahedra that share corners with two equivalent Te(1)O6 octahedra,  a cornercorner with one Li(2)O4 tetrahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one Te(2)O6 octahedra, edges with two equivalent Co(3)O6 octahedra, and edges with two equivalent Cu(3)O6 octahedra. The corner-sharing octahedral tilt angles range from 49-51°. In the third Co site, Co(3) is bonded to one O(10), one O(12), one O(13), one O(15), one O(5), and one O(6) atom to form CoO6 octahedra that share corners with two equivalent Te(1)O6 octahedra,  a cornercorner with one Li(2)O4 tetrahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one Te(2)O6 octahedra, edges with two equivalent Co(2)O6 octahedra, and edges with two equivalent Cu(3)O6 octahedra. The corner-sharing octahedral tilt angles range from 48-51°. There are three inequivalent Cu sites. In the first Cu site, Cu(1) is bonded to one O(14), one O(2), one O(3), one O(4), one O(7), and one O(9) atom to form distorted CuO6 octahedra that share corners with two equivalent Te(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  an edgeedge with one Te(1)O6 octahedra, edges with two equivalent Co(1)O6 octahedra, edges with two equivalent Cu(2)O6 octahedra, and  an edgeedge with one Li(2)O4 tetrahedra. The corner-sharing octahedral tilt angles range from 51-54°. In the second Cu site, Cu(2) is bonded to one O(16), one O(2), one O(3), one O(4), one O(8), and one O(9) atom to form distorted CuO6 octahedra that share corners with two equivalent Te(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  an edgeedge with one Te(1)O6 octahedra, edges with two equivalent Co(1)O6 octahedra, edges with two equivalent Cu(1)O6 octahedra, and  an edgeedge with one Li(2)O4 tetrahedra. The corner-sharing octahedral tilt angles range from 48-55°. In the third Cu site, Cu(3) is bonded to one O(1), one O(11), one O(12), one O(13), one O(5), and one O(6) atom to form CuO6 octahedra that share corners with two equivalent Te(1)O6 octahedra,  a cornercorner with one Li(2)O4 tetrahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one Te(2)O6 octahedra, edges with two equivalent Co(2)O6 octahedra, and edges with two equivalent Co(3)O6 octahedra. The corner-sharing octahedral tilt angles range from 54-55°. There are two inequivalent Te sites. In the first Te site, Te(1) is bonded to one O(1), one O(10), one O(2), one O(6), one O(7), and one O(8) atom to form TeO6 octahedra that share corners with two equivalent Co(2)O6 octahedra, corners with two equivalent Co(3)O6 octahedra, corners with two equivalent Cu(3)O6 octahedra, corners with three equivalent Li(4)O4 tetrahedra,  an edgeedge with one Co(1)O6 octahedra,  an edgeedge with one Cu(1)O6 octahedra, and  an edgeedge with one Cu(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 48-55°. In the second Te site, Te(2) is bonded to one O(11), one O(12), one O(14), one O(15), one O(16), and one O(9) atom to form TeO6 octahedra that share corners with two equivalent Co(1)O6 octahedra, corners with two equivalent Cu(1)O6 octahedra, corners with two equivalent Cu(2)O6 octahedra, corners with three equivalent Li(1)O4 tetrahedra, corners with three equivalent Li(2)O4 tetrahedra,  an edgeedge with one Co(2)O6 octahedra,  an edgeedge with one Co(3)O6 octahedra, and  an edgeedge with one Cu(3)O6 octahedra. The corner-sharing octahedral tilt angles range from 45-55°. There are sixteen inequivalent O sites. In the first O site, O(1) is bonded in a rectangular see-saw-like geometry to one Li(3), one Co(2), one Cu(3), and one Te(1) atom. In the second O site, O(2) is bonded to one Li(4), one Cu(1), one Cu(2), and one Te(1) atom to form distorted OLiCu2Te tetrahedra that share  a cornercorner with one O(13)LiCo2Cu tetrahedra, corners with two equivalent O(4)LiCoCu2 tetrahedra, and  an edgeedge with one O(3)LiCoCu2 tetrahedra. In the third O site, O(3) is bonded to one Li(1), one Co(1), one Cu(1), and one Cu(2) atom to form OLiCoCu2 tetrahedra that share  a cornercorner with one O(11)LiCoCuTe tetrahedra, corners with three equivalent O(4)LiCoCu2 tetrahedra, and  an edgeedge with one O(2)LiCu2Te tetrahedra. In the fourth O site, O(4) is bonded to one Li(3), one Co(1), one Cu(1), and one Cu(2) atom to form OLiCoCu2 tetrahedra that share corners with two equivalent O(2)LiCu2Te tetrahedra and corners with three equivalent O(3)LiCoCu2 tetrahedra. In the fifth O site, O(5) is bonded to one Li(2), one Co(2), one Co(3), and one Cu(3) atom to form OLiCo2Cu tetrahedra that share corners with two equivalent O(11)LiCoCuTe tetrahedra and corners with three equivalent O(13)LiCo2Cu tetrahedra. In the sixth O site, O(6) is bonded in a rectangular see-saw-like geometry to one Li(3), one Co(3), one Cu(3), and one Te(1) atom. In the seventh O site, O(7) is bonded in a 4-coordinate geometry to one Li(4), one Co(1), one Cu(1), and one Te(1) atom. In the eighth O site, O(8) is bonded in a 4-coordinate geometry to one Li(4), one Co(1), one Cu(2), and one Te(1) atom. In the ninth O site, O(9) is bonded in a rectangular see-saw-like geometry to one Li(2), one Cu(1), one Cu(2), and one Te(2) atom. In the tenth O site, O(10) is bonded in a rectangular see-saw-like geometry to one Li(3), one Co(2), one Co(3), and one Te(1) atom. In the eleventh O site, O(11) is bonded to one Li(1), one Co(2), one Cu(3), and one Te(2) atom to form distorted OLiCoCuTe tetrahedra that share  a cornercorner with one O(3)LiCoCu2 tetrahedra, corners with two equivalent O(5)LiCo2Cu tetrahedra, and  an edgeedge with one O(13)LiCo2Cu tetrahedra. In the twelfth O site, O(12) is bonded in a distorted rectangular see-saw-like geometry to one Li(1), one Co(3), one Cu(3), and one Te(2) atom. In the thirteenth O site, O(13) is bonded to one Li(4), one Co(2), one Co(3), and one Cu(3) atom to form OLiCo2Cu tetrahedra that share  a cornercorner with one O(2)LiCu2Te tetrahedra, corners with three equivalent O(5)LiCo2Cu tetrahedra, and  an edgeedge with one O(11)LiCoCuTe tetrahedra. In the fourteenth O site, O(14) is bonded in a distorted rectangular see-saw-like geometry to one Li(2), one Co(1), one Cu(1), and one Te(2) atom. In the fifteenth O site, O(15) is bonded in a rectangular see-saw-like geometry to one Li(1), one Co(2), one Co(3), and one Te(2) atom. In the sixteenth O site, O(16) is bonded in a distorted rectangular see-saw-like geometry to one Li(2), one Co(1), one Cu(2), and one Te(2) atom. is represented by the Crystallographic Information File (CIF) [CIF]
data_Li4Co3Cu3(TeO8)2
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   5.755
_cell_length_b   5.880
_cell_length_c   9.591
_cell_angle_alpha   93.517
_cell_angle_beta   90.185
_cell_angle_gamma   118.527
_symmetry_Int_Tables_number   1
_cell_volume   284.444
_cell_formula_units_Z   1
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Li  Li0  1  0.328  0.672  0.911  1.0
  Li  Li1  1  0.007  0.021  0.988  1.0
  Li  Li2  1  0.002  0.999  0.483  1.0
  Li  Li3  1  0.660  0.304  0.414  1.0
  Co  Co4  1  0.171  0.346  0.217  1.0
  Co  Co5  1  0.835  0.175  0.714  1.0
  Co  Co6  1  0.343  0.172  0.713  1.0
  Cu  Cu7  1  0.663  0.837  0.211  1.0
  Cu  Cu8  1  0.176  0.842  0.211  1.0
  Cu  Cu9  1  0.835  0.667  0.712  1.0
  Te  Te10  1  0.331  0.650  0.488  1.0
  Te  Te11  1  0.667  0.350  0.982  1.0
  O  O12  1  0.675  0.831  0.591  1.0
  O  O13  1  0.483  0.938  0.357  1.0
  O  O14  1  0.327  0.653  0.123  1.0
  O  O15  1  0.007  0.021  0.292  1.0
  O  O16  1  0.012  0.015  0.800  1.0
  O  O17  1  0.177  0.840  0.589  1.0
  O  O18  1  0.453  0.465  0.355  1.0
  O  O19  1  0.023  0.484  0.356  1.0
  O  O20  1  0.836  0.693  0.082  1.0
  O  O21  1  0.163  0.324  0.602  1.0
  O  O22  1  0.962  0.477  0.845  1.0
  O  O23  1  0.488  0.464  0.847  1.0
  O  O24  1  0.661  0.323  0.619  1.0
  O  O25  1  0.844  0.202  0.087  1.0
  O  O26  1  0.524  0.043  0.833  1.0
  O  O27  1  0.348  0.191  0.089  1.0
[/CIF]
.
The material described by Li4Co3Cu3(TeO8)2 is Hausmannite-derived structured and crystallizes in the triclinic P1 space group. There are four inequivalent Li sites. In the first Li site, Li(1) is bonded to one O(11), one O(12), one O(15), and one O(3) atom to form LiO4 tetrahedra that share  a cornercorner with one Co(1)O6 octahedra,  a cornercorner with one Cu(1)O6 octahedra,  a cornercorner with one Cu(2)O6 octahedra, corners with two equivalent Co(2)O6 octahedra, corners with two equivalent Co(3)O6 octahedra, corners with two equivalent Cu(3)O6 octahedra, and corners with three equivalent Te(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 53-68°. In the second Li site, Li(2) is bonded to one O(14), one O(16), one O(5), and one O(9) atom to form distorted LiO4 tetrahedra that share  a cornercorner with one Co(2)O6 octahedra,  a cornercorner with one Co(3)O6 octahedra,  a cornercorner with one Cu(3)O6 octahedra, corners with three equivalent Te(2)O6 octahedra,  an edgeedge with one Co(1)O6 octahedra,  an edgeedge with one Cu(1)O6 octahedra, and  an edgeedge with one Cu(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 56-68°. In the third Li site, Li(3) is bonded in a rectangular see-saw-like geometry to one O(1), one O(10), one O(4), and one O(6) atom. In the fourth Li site, Li(4) is bonded to one O(13), one O(2), one O(7), and one O(8) atom to form LiO4 tetrahedra that share  a cornercorner with one Co(2)O6 octahedra,  a cornercorner with one Co(3)O6 octahedra,  a cornercorner with one Cu(3)O6 octahedra, corners with two equivalent Co(1)O6 octahedra, corners with two equivalent Cu(1)O6 octahedra, corners with two equivalent Cu(2)O6 octahedra, and corners with three equivalent Te(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 50-68°. There are three inequivalent Co sites. In the first Co site, Co(1) is bonded to one O(14), one O(16), one O(3), one O(4), one O(7), and one O(8) atom to form CoO6 octahedra that share corners with two equivalent Te(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  an edgeedge with one Te(1)O6 octahedra, edges with two equivalent Cu(1)O6 octahedra, edges with two equivalent Cu(2)O6 octahedra, and  an edgeedge with one Li(2)O4 tetrahedra. The corner-sharing octahedral tilt angles range from 45-48°. In the second Co site, Co(2) is bonded to one O(1), one O(10), one O(11), one O(13), one O(15), and one O(5) atom to form CoO6 octahedra that share corners with two equivalent Te(1)O6 octahedra,  a cornercorner with one Li(2)O4 tetrahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one Te(2)O6 octahedra, edges with two equivalent Co(3)O6 octahedra, and edges with two equivalent Cu(3)O6 octahedra. The corner-sharing octahedral tilt angles range from 49-51°. In the third Co site, Co(3) is bonded to one O(10), one O(12), one O(13), one O(15), one O(5), and one O(6) atom to form CoO6 octahedra that share corners with two equivalent Te(1)O6 octahedra,  a cornercorner with one Li(2)O4 tetrahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one Te(2)O6 octahedra, edges with two equivalent Co(2)O6 octahedra, and edges with two equivalent Cu(3)O6 octahedra. The corner-sharing octahedral tilt angles range from 48-51°. There are three inequivalent Cu sites. In the first Cu site, Cu(1) is bonded to one O(14), one O(2), one O(3), one O(4), one O(7), and one O(9) atom to form distorted CuO6 octahedra that share corners with two equivalent Te(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  an edgeedge with one Te(1)O6 octahedra, edges with two equivalent Co(1)O6 octahedra, edges with two equivalent Cu(2)O6 octahedra, and  an edgeedge with one Li(2)O4 tetrahedra. The corner-sharing octahedral tilt angles range from 51-54°. In the second Cu site, Cu(2) is bonded to one O(16), one O(2), one O(3), one O(4), one O(8), and one O(9) atom to form distorted CuO6 octahedra that share corners with two equivalent Te(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  an edgeedge with one Te(1)O6 octahedra, edges with two equivalent Co(1)O6 octahedra, edges with two equivalent Cu(1)O6 octahedra, and  an edgeedge with one Li(2)O4 tetrahedra. The corner-sharing octahedral tilt angles range from 48-55°. In the third Cu site, Cu(3) is bonded to one O(1), one O(11), one O(12), one O(13), one O(5), and one O(6) atom to form CuO6 octahedra that share corners with two equivalent Te(1)O6 octahedra,  a cornercorner with one Li(2)O4 tetrahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one Te(2)O6 octahedra, edges with two equivalent Co(2)O6 octahedra, and edges with two equivalent Co(3)O6 octahedra. The corner-sharing octahedral tilt angles range from 54-55°. There are two inequivalent Te sites. In the first Te site, Te(1) is bonded to one O(1), one O(10), one O(2), one O(6), one O(7), and one O(8) atom to form TeO6 octahedra that share corners with two equivalent Co(2)O6 octahedra, corners with two equivalent Co(3)O6 octahedra, corners with two equivalent Cu(3)O6 octahedra, corners with three equivalent Li(4)O4 tetrahedra,  an edgeedge with one Co(1)O6 octahedra,  an edgeedge with one Cu(1)O6 octahedra, and  an edgeedge with one Cu(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 48-55°. In the second Te site, Te(2) is bonded to one O(11), one O(12), one O(14), one O(15), one O(16), and one O(9) atom to form TeO6 octahedra that share corners with two equivalent Co(1)O6 octahedra, corners with two equivalent Cu(1)O6 octahedra, corners with two equivalent Cu(2)O6 octahedra, corners with three equivalent Li(1)O4 tetrahedra, corners with three equivalent Li(2)O4 tetrahedra,  an edgeedge with one Co(2)O6 octahedra,  an edgeedge with one Co(3)O6 octahedra, and  an edgeedge with one Cu(3)O6 octahedra. The corner-sharing octahedral tilt angles range from 45-55°. There are sixteen inequivalent O sites. In the first O site, O(1) is bonded in a rectangular see-saw-like geometry to one Li(3), one Co(2), one Cu(3), and one Te(1) atom. In the second O site, O(2) is bonded to one Li(4), one Cu(1), one Cu(2), and one Te(1) atom to form distorted OLiCu2Te tetrahedra that share  a cornercorner with one O(13)LiCo2Cu tetrahedra, corners with two equivalent O(4)LiCoCu2 tetrahedra, and  an edgeedge with one O(3)LiCoCu2 tetrahedra. In the third O site, O(3) is bonded to one Li(1), one Co(1), one Cu(1), and one Cu(2) atom to form OLiCoCu2 tetrahedra that share  a cornercorner with one O(11)LiCoCuTe tetrahedra, corners with three equivalent O(4)LiCoCu2 tetrahedra, and  an edgeedge with one O(2)LiCu2Te tetrahedra. In the fourth O site, O(4) is bonded to one Li(3), one Co(1), one Cu(1), and one Cu(2) atom to form OLiCoCu2 tetrahedra that share corners with two equivalent O(2)LiCu2Te tetrahedra and corners with three equivalent O(3)LiCoCu2 tetrahedra. In the fifth O site, O(5) is bonded to one Li(2), one Co(2), one Co(3), and one Cu(3) atom to form OLiCo2Cu tetrahedra that share corners with two equivalent O(11)LiCoCuTe tetrahedra and corners with three equivalent O(13)LiCo2Cu tetrahedra. In the sixth O site, O(6) is bonded in a rectangular see-saw-like geometry to one Li(3), one Co(3), one Cu(3), and one Te(1) atom. In the seventh O site, O(7) is bonded in a 4-coordinate geometry to one Li(4), one Co(1), one Cu(1), and one Te(1) atom. In the eighth O site, O(8) is bonded in a 4-coordinate geometry to one Li(4), one Co(1), one Cu(2), and one Te(1) atom. In the ninth O site, O(9) is bonded in a rectangular see-saw-like geometry to one Li(2), one Cu(1), one Cu(2), and one Te(2) atom. In the tenth O site, O(10) is bonded in a rectangular see-saw-like geometry to one Li(3), one Co(2), one Co(3), and one Te(1) atom. In the eleventh O site, O(11) is bonded to one Li(1), one Co(2), one Cu(3), and one Te(2) atom to form distorted OLiCoCuTe tetrahedra that share  a cornercorner with one O(3)LiCoCu2 tetrahedra, corners with two equivalent O(5)LiCo2Cu tetrahedra, and  an edgeedge with one O(13)LiCo2Cu tetrahedra. In the twelfth O site, O(12) is bonded in a distorted rectangular see-saw-like geometry to one Li(1), one Co(3), one Cu(3), and one Te(2) atom. In the thirteenth O site, O(13) is bonded to one Li(4), one Co(2), one Co(3), and one Cu(3) atom to form OLiCo2Cu tetrahedra that share  a cornercorner with one O(2)LiCu2Te tetrahedra, corners with three equivalent O(5)LiCo2Cu tetrahedra, and  an edgeedge with one O(11)LiCoCuTe tetrahedra. In the fourteenth O site, O(14) is bonded in a distorted rectangular see-saw-like geometry to one Li(2), one Co(1), one Cu(1), and one Te(2) atom. In the fifteenth O site, O(15) is bonded in a rectangular see-saw-like geometry to one Li(1), one Co(2), one Co(3), and one Te(2) atom. In the sixteenth O site, O(16) is bonded in a distorted rectangular see-saw-like geometry to one Li(2), one Co(1), one Cu(2), and one Te(2) atom. is represented by the Crystallographic Information File (CIF) [CIF]
data_Li4Co3Cu3(TeO8)2
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   5.755
_cell_length_b   5.880
_cell_length_c   9.591
_cell_angle_alpha   93.517
_cell_angle_beta   90.185
_cell_angle_gamma   118.527
_symmetry_Int_Tables_number   1
_cell_volume   284.444
_cell_formula_units_Z   1
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Li  Li0  1  0.328  0.672  0.911  1.0
  Li  Li1  1  0.007  0.021  0.988  1.0
  Li  Li2  1  0.002  0.999  0.483  1.0
  Li  Li3  1  0.660  0.304  0.414  1.0
  Co  Co4  1  0.171  0.346  0.217  1.0
  Co  Co5  1  0.835  0.175  0.714  1.0
  Co  Co6  1  0.343  0.172  0.713  1.0
  Cu  Cu7  1  0.663  0.837  0.211  1.0
  Cu  Cu8  1  0.176  0.842  0.211  1.0
  Cu  Cu9  1  0.835  0.667  0.712  1.0
  Te  Te10  1  0.331  0.650  0.488  1.0
  Te  Te11  1  0.667  0.350  0.982  1.0
  O  O12  1  0.675  0.831  0.591  1.0
  O  O13  1  0.483  0.938  0.357  1.0
  O  O14  1  0.327  0.653  0.123  1.0
  O  O15  1  0.007  0.021  0.292  1.0
  O  O16  1  0.012  0.015  0.800  1.0
  O  O17  1  0.177  0.840  0.589  1.0
  O  O18  1  0.453  0.465  0.355  1.0
  O  O19  1  0.023  0.484  0.356  1.0
  O  O20  1  0.836  0.693  0.082  1.0
  O  O21  1  0.163  0.324  0.602  1.0
  O  O22  1  0.962  0.477  0.845  1.0
  O  O23  1  0.488  0.464  0.847  1.0
  O  O24  1  0.661  0.323  0.619  1.0
  O  O25  1  0.844  0.202  0.087  1.0
  O  O26  1  0.524  0.043  0.833  1.0
  O  O27  1  0.348  0.191  0.089  1.0
[/CIF]
.